- About this Journal ·
- Abstracting and Indexing ·
- Advance Access ·
- Aims and Scope ·
- Article Processing Charges ·
- Articles in Press ·
- Author Guidelines ·
- Bibliographic Information ·
- Citations to this Journal ·
- Contact Information ·
- Editorial Board ·
- Editorial Workflow ·
- Free eTOC Alerts ·
- Publication Ethics ·
- Reviewers Acknowledgment ·
- Submit a Manuscript ·
- Subscription Information ·
- Table of Contents

Advances in Physical Chemistry

Volume 2011 (2011), Article ID 786759, 20 pages

http://dx.doi.org/10.1155/2011/786759

## (Photo)electrochemical Methods for the Determination of the Band Edge Positions of TiO_{2}-Based Nanomaterials

^{1}Faculty of Chemistry and Biochemistry, Ruhr University Bochum, Universitätstr 150, NC4/073, D-44780 Bochum, Germany^{2}Materials Research Department, Ruhr University Bochum, D-44801 Bochum, Germany^{3}Research Department Interfacial Systems Chemistry, Ruhr University Bochum, D-44801 Bochum, Germany

Received 30 September 2011; Accepted 15 December 2011

Academic Editor: Konstantin Neyman

Copyright © 2011 Radim Beranek. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.

#### Abstract

TiO_{2}-based nanomaterials play currently a major role in the development of novel photochemical systems and devices. One of the key parameters determining the photoactivity of TiO_{2}-based materials is the position of the band edges. Although its knowledge is an important prerequisite for understanding and optimizing the performance of photochemical systems, it has been often rather neglected in recent research, particularly in the field of heterogeneous photocatalysis. This paper provides a concise account of main methods for the determination of the position of the band edges, particularly those suitable for measurements on nanostructured materials. In the first part, a survey of key photophysical and photochemical concepts necessary for understanding the energetics at the semiconductor/solution interface is provided. This is followed by a detailed discussion of several electrochemical, photoelectrochemical, and spectroelectrochemical methods that can be applied for the determination of band edge positions in compact and nanocrystalline thin films, as well as in nanocrystalline powders.

#### 1. Introduction

Although first scientific reports of photoinduced effects of titanium dioxide on chemical reactions were available already more than ninety years ago [1–8], it was first in the 1970s that potential practical applications of TiO_{2} photoelectrochemistry and photocatalysis have been fully recognized. This was particularly due to the pioneering work of Fujishima and Honda on solar-driven water splitting into hydrogen and oxygen using a TiO_{2} photoanode [9–11], which promised utilization of TiO_{2}-based materials for solar energy conversion and storage [12–16]. In following years further photochemical applications of TiO_{2} have been realized, most of them motivated particularly by the advantageous combination of its low cost, nontoxicity, and excellent stability against photocorrosion. One important example is the rapidly growing field of heterogeneous photocatalysis [17–25], in which TiO_{2} has been successfully employed in photooxidation reactions utilizing aerobic oxygen for the complete removal of pollutants from water and air [17–22, 24–39], in preparation of superhydrophilic and antifogging surfaces [40–43], in photocatalytic organic syntheses [44–49], or in antitumor medicinal applications [50–54].

Importantly, although the bandgap energy of TiO_{2} is rather large (for anatase 3.2 eV; ~ 390 nm) and direct band-to-band excitation can therefore only be achieved by high-energy UV light, the utilization of TiO_{2} is not confined to UV-light-driven applications. Drawing on the fundamental studies on dye sensitization of other wide bandgap semiconductors (ZnO, SnO_{2}) in the 1960s [55–59], attaching visible-light-absorbing organic dyes to the surface of TiO_{2} [60, 61] has led to fabrication of regenerative dye-sensitized solar cells with the overall solar conversion efficiencies exceeding 10% [62–64]. Other sensitization approaches utilize chromophores like semiconductor quantum dots [65–70], plasmonic metal nanocrystals [71–75], simple coordination compounds like chloroplatinate (IV) complexes [29, 32, 76] or ferrocyanide ions [77–79], stable polymeric compounds [38, 39, 80–83], or metal ions (, ) grafted onto the TiO_{2} surface [84, 85]. In contrast to these *surface*-confined sensitization protocols, *bulk*-doping of TiO_{2} has also attracted significant interest. In the latter approach, transition metals [86–88] or main-group elements like carbon [35, 89], nitrogen [31, 90–97], and sulfur [98, 99] are introduced into the lattice of titania resulting in formation of intrabandgap donor and acceptor levels, allowing thus for visible light ( nm) excitation. Apart from the fields of solar cells and photocatalysis, the visible light-responsive TiO_{2} materials opened up a route for further developments including photoelectrochemistry-based sensors [100, 101] and light-addressable photoelectrochemical optoelectronic devices [102–106].

Obviously, many applications can benefit from TiO_{2} materials with fine-tuned structural and surface characteristics. Particularly nanostructured and mesoporous materials with a large surface-to-volume ration are highly profitable for most applications. This motivated the development of a great variety of synthetic protocols which allow for fabrication of TiO_{2} with well-defined morphologies on the micro- and nanoscale. These include, for example, nanoporous spheres [107], nanotubes [108, 109], hierarchical nanodendrite-nanoparticle composites [110], organized mesoporous TiO_{2} films with controlled crystallinity [111, 112], nanoparticles with distinct crystal facets [113, 114], or TiO_{2} inverse opals materials exhibiting photonic bandgap [115–117]. In addition, the modification of surface catalytic properties has been achieved, for instance, by coupling TiO_{2} with gold nanostructures [118], graphene [119], or reduced graphene oxide [120, 121].

Notwithstanding the huge variety of different TiO_{2}-based materials, it is important to realize that the fundamental basis for all photochemical applications of TiO_{2} is its *semiconducting* electronic structure [122, 125–129]. In other words, it is the energy band structure that underlies the photoactivity of TiO_{2}-based materials, whereby the position of the band edges on the electrochemical potential scale exerts a crucial influence on the operation of the photochemical system. This can be well exemplified in Figure 1. A typical photocatalytic reaction at small TiO_{2} particles is initiated by absorption of a UV light photon, whereby a pair of charges is generated—an electron in the conduction band and a hole in the valence band (Figure 1(a)). The photogenerated charges can either recombine or undergo an interfacial electron transfer process, whereby the electron reduces an electron acceptor species A to a primary reduction product A^{−•}, and the hole oxidizes an electron donor species to D^{+•}. Hence, for example, during a typical photocatalytic oxidation of organic pollutants on TiO_{2} in aqueous solutions, the reacting holes are scavenged either directly by the pollutant or by adsorbed hydroxyl ions to produced hydroxyl radicals which can then oxidize the pollutant due to their high oxidizing power. Simultaneously, the photogenerated electrons reduce molecular oxygen to a superoxide radical ( V versus NHE [130]) which can then undergo further reactions to produce hydroxyl radicals [17, 131–134]. It is obvious that the positions of the conduction and valence band edges are of crucial importance here since these give information on the reductive and oxidative power of photogenerated electrons and holes, respectively. Interestingly, the product of the one-hole oxidation of some electron donors—like, for example, the methoxy radical as a primary oxidation product of methanol (Figure 1(b))—is a very strong reducing agent that can inject an electron into the conduction band of TiO_{2} and is thereby further oxidized to formaldehyde. Since this generation of *two* electrons in the conduction band upon absorption of *one* photon has been first observed during photocurrent measurements, it has been coined as the *photocurrent-doubling effect* (photocurrent-multiplication effect) [125]. It goes without saying that the position of the conduction band edge on the potential scale will again play an essential role for the efficiency of the electron injection in such a case. Obviously, similar consideration will be also valid in cases when the photoprocess is based on light absorption by a sensitizer, typically a dye (Figure 1(c)). Here, the dye gets into an excited state from which it injects an electron into the conduction band of a semiconductor and is thereby oxidized. Alternatively to this *photoinduced electron transfer* scenario, in case of a strong coupling between the sensitizer and TiO_{2} the so-called *direct optical electron transfer* from the chromophore’s HOMO into the conduction band of TiO_{2} can occur, as known, for example, for TiO_{2} covalently sensitized with catechol [135–137], chlorophenols [138, 139], or polymeric compounds [140]. In case of TiO_{2}-assisted photooxidation reactions based on sensitization, one often speaks about “*indirect* photocatalysis” since the reaction is not initiated through direct photon absorption by TiO_{2} (“*direct* photocatalysis”; Figure 1(a)), but instead indirectly, through the light absorption by a dye [24, 25, 34, 37]. At any rate, the position of the conduction band edge must be positive enough in order to allow for the injection from the dye, and at the same time negative enough, in order to allow for further electron transfer to suitable acceptors in the solution (e.g., oxygen).

From the above stated, it is clear that the positions of the band edges exert a crucial influence on the photoactivity of TiO_{2}-based materials. In this context, it is rather surprising that the determination of the band edge position is still only very rarely directly addressed experimentally, particularly in research directed to the development of new photocatalysts. This causes a serious lacuna in our understanding of the photoactivity of such novel materials since the position of the band edges in many cases cannot be simply predicted or taken from the literature data. This is due to the fact that the band edge positions of TiO_{2}-based materials will normally depend on surface charging. This will be highly dependent not only on the ionic conditions in a concrete electrolyte (pH, specific adsorption of ions), but also on the surface structure and composition of the material, which, in turn, will depend on the particular synthetic strategy used for the fabrication. The aim of this paper is to review various methods for the measurement of the band edge positions of TiO_{2}-based materials. The focus will be particularly on nanostructured materials used in photocatalysis and other applications operating in aqueous electrolytes. The paper will start with a short summary of some fundamental concepts of semiconductor photophysics and photochemistry (quasi-Fermi levels, flatband potential, pH dependence of band edges) that are directly relevant for understanding the problem of band edge determination. Then, a theoretical approach to the calculation of the band edges position, together with the application of conventional spectroscopic and contact potential difference measurements, will be shortly discussed. This will be followed by a detailed discussion of various electrochemical, photoelectrochemical, and spectroelectrochemical methods that can be applied to measurements on TiO_{2}-based materials in the form of thin compact films, porous nanocrystalline layers, and nanocrystalline powders.

#### 2. Theory and Fundamental Concepts

##### 2.1. Quasi-Fermi Levels and Flatband Potential

TiO_{2} is typically found in one of its three main crystal structures: rutile (tetragonal), anatase (tetragonal), or brookite (orthorhombic). Out of these, anatase is the polymorph most widely used for photocatalytic and photoelectrochemical purposes. It is noteworthy that the conduction band edge states have predominantly the Ti 3*d* character, while the valence-band edge states have the O 2*p* character. Importantly, due to its inherent nonstoichiometry (oxygen vacancies), TiO_{2} is typically a rather heavily doped n-type semiconductor. This means that its *Fermi level *() is typically right below the conduction band edge (). From the thermodynamic point of view, the Fermi level is the electrochemical potential of the electron in the solid. Equivalently, from the statistical point of view, the Fermi level is the energy at which the probability of an energy level being occupied by an electron (the Fermi function) is 0.5 (Note, however, that this does not imply that the level at the Fermi energy is populated by electrons because the population depends upon the product of the Fermi function and the electron density of states). Hence, the Fermi level describes the occupation of energy levels in a semiconductor at thermodynamic equilibrium. However, the condition of thermodynamic equilibrium is not always fulfilled—particularly when excess electrons and holes are photogenerated under illumination or injected under electric bias. Accordingly, the electron and hole densities in the conduction and valence band are not described by the same Fermi level but by a *quasi*-Fermi level of electrons and a *quasi*-Fermi level of holes , respectively (Figure 2) [125, 126, 128]. In general, the density of majority carriers (electrons in case of TiO_{2}) does not significantly increase upon illumination and the quasi-Fermi level for majority carriers is normally almost the same as the Fermi level at equilibrium. In contrast, the density of minority carriers (holes) can be increased by many orders of magnitude, which then leads to a shift of the quasi-Fermi level of holes downwards to the vicinity of the valence band edge.

It should be also noted that the generation of electron-hole pairs often occurs locally near the semiconductor surface due to the small penetration depth of light, which leads to variations in the quasi-Fermi level of holes with the distance from the surface (Figure 2(c)). Importantly, in case of heavily doped n-type metal oxides like TiO_{2}, the lower conduction band edge, , practically merges with the quasi-Fermi level for electrons, , () [125]. Therefore, as will be discussed below in more detail, the determination of the conduction band edge often translates into the measurement of the position of the quasi-Fermi level of electrons. Once this is known, the position of the valence band edge can be simply calculated by adding the value of bandgap energy, that is, typically determined by optical [128, 141–151] or photoelectrochemical methods [152–156].

Another important concept, particularly in case of compact flat TiO_{2} films that behave similarly to single crystal semiconductors, is the *flatband potential*. First, let us consider the energetic situation at the n-type semiconductor/electrolyte interface before and after the contact of the two phases (Figure 3). After the contact of the semiconductor surface with the electrolyte, the thermodynamic equilibrium on both sides of the interface must be established [125–128, 157]. In other words, the Fermi level of the semiconductor is adjusted to the Fermi level of the electrolyte . The latter can be considered nearly constant because the number of available states per unit energy in the solution typically far exceeds the number present in a semiconductor. This equilibration happens through electron transfer across the interface, which results in formation of the space-charge layer—also called the “depletion layer” since the surface region of the semiconductor is depleted of its majority carriers. It is important to realize that, in the case of an n-type semiconductor, this interfacial charge-transfer process produces an excess of positive charges in the semiconductor (immobile charges of ionized donors) and an excess of negative charges in the electrolyte. With more electrons exchanged, the electric field of the negative charges on the solution side hinders further electron transfer so that the equilibrium is established in which no net charge flow occurs. As a consequence, the bands are bent upwards, which can be understood in terms of a continuously growing barrier for interfacial electron transfer when moving from the bulk of the semiconductor to the interface due to the continuously less efficient screening of the negative charges in the solution by the positive charges in the depletion layer [127]. The height of the barrier is the energy difference between the conduction band edge in the bulk () semiconductor and the conduction band edge at the surface () and corresponds to the potential drop in the space-charge layer .

The charge distribution scenario at semiconductor/electrolyte interface is summarized in Figure 4. Importantly, three distinct double layers can be distinguished at the interface. First, it is the semiconductor space-charge layer with positive charges in the form of ionized donors and the counter negative charge located at the surface. The second one is the Helmholtz double layer consisting of the inner Helmholtz plane (IHP) and the outer Helmholtz plane (OHP). The first is located at the semiconductor surface, and the charge is in the surface states or at the location of specifically adsorbed ions, whereas the latter denotes the position of the closest approach of hydrated mobile ions. Finally, there is the Gouy-Chapman layer which is extended region with an excess of free ions of one sign. Essentially, the double layers act as parallel-plate capacitors connected in series with capacitances , , and representing the capacitance of the space-charge layer, the capacitance of the Helmholtz double layer, and the capacitance of the Gouy-Chapman layer, respectively, whereby can be typically neglected for electrolytes containing relatively high concentrations of redox species (Figure 4(d)).

The simplest quantitative description of the situation at the semiconductor/electrolyte interface [125–129, 157] is analogous to the Schottky diode model and is based on the following assumptions: (i) ideal, crystalline semiconductor, homogeneous donor level near the conduction band (oxygen vacancies in the form of sites in case of TiO_{2}) with all donors ionized (all the electrons from the donors have been thermally excited to the conduction band); (ii) no surface states; (iii) potential drop in the Helmholtz layer can be neglected. The potential and charge distribution within the space-charge layer can be then described by a one-dimensional Poisson equation:
where is potential, *x* is distance, and are the relative permittivity of the semiconductor and the permittivity of vacuum, respectively, and is the volume charge density. After two integrations assuming (*q* is the elementary charge; *N* is the doping concentration) and the boundary conditions for and for (see [125, 126, 128] for details), one obtains the following relation for the width of the space-charge layer *W*:
where is the potential drop in the space-charge layer which can be obtained as

or
where is externally applied potential and is the potential at which and the bands in the semiconductor are “flat” (*flatband potential*). It is now clear that the value of is of fundamental significance since it gives a direct information on the position of the conduction band edge at the n-type semiconductor’s surface (), assuming that the difference between and is very small for doped semiconductors. In other words, the determination of the conduction band edge of thin compact TiO_{2} films often translates into the measurement of the flatband potential (for more details, see below). However, it should be emphasized that, in the context of nanomaterials, the above described formalism applies only to thin compact highly doped TiO_{2} films that behave in a manner similar to compact crystalline semiconductors. In contrast, in small TiO_{2} particles and in highly porous nanocrystalline electrodes, the formation of the space-charge layer is improbable due to the very small crystallite size [158–163]. In other words, the nearly depleted small TiO_{2} crystals do not contain enough electrons in order to create an effective space-charge layer. Several methods suitable for the determination of band edges in such nanocrystalline systems will be presented below.

##### 2.2. pH Dependence of the Position of Band Edges

The position of the band edges at the surface () is determined by the charge at the surface, that is, by the potential drop in the Helmholtz layer :
where is the position (on the energy scale) of the conduction band edge at the surface at . The Helmholtz double layer at semiconductors is typically determined through adsorption and desorption processes, which is particularly true for ionic oxide semiconductors like TiO_{2} in aqueous electrolytes. In this case, the protons and hydroxyl groups play an essential role while the specific adsorption of other ions can be in most cases neglected.

In essence, the lattice Ti atoms act as Lewis acid sites and make the adsorption of hydroxyl ions possible, whereas the bridging lattice oxygen attracts protons and acts thereby as a Lewis base site. Hence, depending on the pH, the semiconductor surface becomes charged either positively or negatively (Figure 5). The pH value at which the net surface charge is zero is called the isoelectric point (pH_{IEP}) or the point of zero zeta potential (pzzp). (Here, it should be noted that pH_{IEP} and pzzp are *not* necessarily identical with the point of zero charge, pzc, that denotes the pH value at which H^{+} and OH^{−} are adsorbed in equal amounts; when other ions than H^{+} and OH^{−} are present and influence the charging of the surface, the pzc and the pH_{IEP} are not equal). The pH dependence of the conduction band edge at the surface can be then derived as follows [125]. Assuming , we obtain the following equilibrium reaction:
where is a hydroxonium ion in the solution and is an adsorbed proton. The equilibrium is described by
where is the free Gibbs energy, is the potential drop in the Helmholtz double layer, and is a constant (assuming that varies linearly with ). Assuming , the following relation can be obtained:
in which (pH_{IEP}) assuming at pH_{IEP}. By combining (5) and (8), we obtain now
Accordingly, with increasing pH, the band edges at the surface shift to higher energies (on the energy scale), that is, to more cathodic potentials (on the electrode potential scale), whereby the shift at 298 K is typically ~ 0.059 V/pH unit.

##### 2.3. Non-Ideal Behavior due to Surface States

The theoretical considerations described in Sections 2.1 and 2.2 assume that the charging of the semiconductor surface (i.e., the position of its band edges) is independent of the applied potential (applied bias voltage is effectively “consumed” within the space-charge layer) or irradiation (minority charge carriers are efficiently scavenged by species in the electrolyte). However, many semiconductors can have localized surface energy levels in the bandgap—the so-called “surface states”—which are typically related to crystal defects or surface damage, or they may result from surface reactions occurring in the dark or under illumination [128, 168, 169]. Obviously, relatively high density of surface states can be present at the surface of doped or surface-modified TiO_{2}-based materials. It is important to realize that the presence of surface states can have significant effects on the position of band edges. During electrode polarization, the Fermi level can match the energy level of the surface states, which will lead to their charging. This might result in the change of the net charge at the surface (i.e., change in the potential drop across the Helmholtz layer), which will cause a shift of the band edge positions. Similarly, during irradiation, the surface states may act as traps for photogenerated charge carriers. Thus, for example, the minority charge carriers (holes in case of n-type TiO_{2}) or charged surface intermediates can accumulate at the surface, which will again lead to changes in the surface charging and result in “unpinning” of band edges [170]. In photoelectrochemical experiments, these problems can be to some extent avoided by adding efficient scavengers of minority charge carriers into the electrolyte [171].

##### 2.4. Theoretical Predictions of the Position of Band Edges

Butler and Ginley introduced a theoretical approach for the prediction of the position of band edges using the following relation [125, 164]:
where is the energy of free electrons on the hydrogen scale (), is the bandgap energy, and is the Sanderson electronegativity of the semiconductor, expressed as the geometric mean of the electronegativities of the constituent atoms, which are defined after Mulliken as the arithmetic mean of the atomic electron affinity and the first ionization energy (both in eV). Calculation for TiO_{2} gives , which (assuming for anatase) yields the value of of +0.24 eV (relative to standard hydrogen electrode on the energy scale, i.e., −0.24 V versus NHE on the electrode potential scale). Interestingly, this result is only by ~0.1 V more negative than experimental results obtained by measurements on anatase single crystals [172]. Although several more sophfisticated theories based on DFT calculations have been developed recently [173–175], the theoretical predictions cannot be always expected to yield sufficiently reliable results, mainly in case of doped and surface-modified TiO_{2}-based materials.

##### 2.5. Spectroscopic and Contact Potential Difference Techniques

Obviously, some key quantities related to the positions of energy bands (see Figure 3) can be obtained also from spectroscopic and contact potential difference measurements performed in a “dry” (or “semidry”) state. Thus, for example, the ionization energy of the semiconductor (, defined as the energy needed to excite an electron from the valence band edge at the surface to the local vacuum level) can be measured by photoemission spectroscopy (e.g., UPS) [176]. On the other hand, the Kelvin probe method can be used for determination of the contact potential difference (*CPD*), that is, of the difference between the work function of a semiconductor and the work function of the metal tip of the probe (with known position on the energy vacuum scale) [177]. Moreover, the latter technique can be combined with illumination in the so-called surface photovoltage spectroscopy in which the changes of the *CPD* (i.e., of surface voltage) upon illumination are measured [178, 179]. Importantly, the saturation surface photovoltage is then directly related to the difference of the position of the Fermi level in the dark and the position of the *quasi*-Fermi level under illumination [180]. As an alternative to the Kelvin probe technique, the surface photovoltage can be also measured directly utilizing a metal-insulator-semiconductor structure and using chopped illumination in conjunction with lock-in detection of the surface photovoltage signal [178, 179]. Importantly in the context of this paper, a standard surface photovoltage measurement can typically be performed also in the presence of adsorbents like water molecules at the surface of the semiconductor (“semidry” state) [181]. Moreover, the Kelvin probe measurements of photoelectrodes immersed into electrolyte have been reported, whereby the electrode and the electrolyte were separated from the Kelvin probe tip by a very thin glass plate [182]. This method has been, for example, used for the estimation of the quasi-Fermi level in the TiO_{2} nanocrystalline layers of dye-sensitized solar cells [183].

A more detailed discussion of these approaches is beyond the scope of this paper. Herein, we deal mainly with TiO_{2}-based materials for use in photocatalysis and photoelectrochemistry and the focus is on electrochemical and photoelectrochemical methods addressing the band energetics directly under operational conditions in (mostly aqueous) solutions. As already mentioned, experimentally the problem of determination of the band edge position is typically addressed by the measurement of the flatband potential or of the quasi-Fermi level. Several electrochemical, photoelectrochemical, and spectroelectrochemical methods will be now discussed in more detail.

#### 3. (Photo)electrochemical Methods

##### 3.1. Capacitance Measurements on Thin Compact Films

As already noted above, since thin compact TiO_{2} films (e.g., dense anodic TiO_{2} films on Ti) behave similarly to conventional macroscopic semiconductor electrodes, the Schottky formalism can be applied and their conduction band edge potential can be measured as the flatband potential. Using the model of a parallel-plate capacitor, the Mott-Schottky relation can be obtained from (2):
The interface double layer capacitances and can be treated as two capacitors connected in series (Figure 4(d)). The overall capacitance is then given by
Under some conditions (a single crystal-like behavior, moderate doping, surface states neglected), it can be assumed that the width of the space-charge layer is much larger than the width of the Helmholtz layer, which yields and, accordingly, .

A widely used technique for the determination of the capacitance is the measurement of impedance. In these experiments, an *ac*-voltage signal of small amplitude is used for the perturbation of the sample. From the current response, the impedance value and the phase shift can be determined. There are essentially two common impedance techniques, which enable us to get information about the capacitive behavior of a system. Either the impedance spectrum for a certain range of frequencies is measured (usually under potentiostatic conditions) or one particular frequency is chosen and the impedance is measured at constant frequency in dependence on the applied potential. Using the latter technique, the capacitance of the space-charge layer can be calculated from the imaginary part of measured impedance:
where denotes the imaginary part of impedance, *i *is imaginary unit, and is the frequency of *ac*-voltage signal. For determination of , a relatively high frequency is usually chosen and a simple equivalent circuit (neglecting the capacitive contribution of other elements) is employed for the interpretation of measured data.

From the resulting Mott-Schottky plot ( versus *E*; see Figure 6), the flatband potential and the doping density can be now obtained as the intercept with the -axis and from the slope of the linear part. The value of the flatband potential from capacitance measurements on single-crystal anatase is reported to be −0.16 V versus NHE (pH 0) with a Nernstian behavior exhibiting a shift of −0.06 V/pH unit [172]. However, it should be noted that the impedance response of the probed system often contains all contributions of the experimental setup, including back contact capacitance, sample resistance, electrolyte resistance, capacitance and resistance of Helmholtz layer and of surface states, which sometimes causes non-ideal behavior and makes it difficult to obtain reliable values of (see Figure 6) when using highly simplified equivalent circuits as in Figure 4(d).

##### 3.2. Photocurrent Onset Measurements

Another common method for the determination of the position of the conduction band edge is a measurement of the potential dependence of photocurrent. The principle of photocurrent generation is explained in Figure 7. If a compact n-type semiconductor (like, e.g., a dense anodic TiO_{2} film on Ti) immersed in the electrolyte under depletion conditions is irradiated with light of higher energy than that of its bandgap, electron-hole pairs are generated and separated in the potential gradient of the space-charge layer (Figure 7(a)). In the case of an n-type semiconductor, this potential gradient drives photogenerated holes toward the semiconductor/electrolyte interface and electrons toward the interior of the electrode and from there to the electrical connection to the external circuit. Accordingly, anodic (positive) photocurrents are typically observed at TiO_{2} photoelectrodes. Obviously, if we sweep the potential of the photoelectrode in cathodic direction (upwards on the potential scale), the band bending will be less and less pronounced. The diminished potential gradient and thickness of the space-charge layer will lead to enhanced recombination of photogenerated charges, which will, in turn, lead to constant decrease of photocurrents during the cathodic potential sweep. Finally, at the flatband potential, the photocurrent should disappear totally [184]. Hence, this so-called “photocurrent onset” potential can be considered to coincide with the flatband potential and to merge practically with the conduction band edge.

Interestingly, similar principle applies also in case of nanocrystalline porous electrodes, in which the photogenerated charge separation is not controlled by the potential gradient over the space-charge region since the crystallite size is too small to support an effective depletion layer [158, 159]. Here, the photocurrent is determined by the efficiency of photogenerated electron/hole transfer at the semiconductor/electrolyte and semiconductor/substrate interface [160–163]. This is schematically illustrated in Figure 7(b) which shows the mechanism of photocurrent generation at TiO_{2} particles deposited on the conductive glass substrate (e.g., ITO). Assuming the presence of suitable redox species in the electrolyte, photogenerated holes immediately react with these at the surface of the particles. The photogenerated electrons can be transferred to the underlying conductive glass substrate, assuming that the Fermi level of the conductive glass is positive enough. Hence again, by moving the Fermi level of the ITO electrode cathodically, we should observe the disappearance of photocurrents when the potential of the underlying electrode (the Fermi level of ITO) reaches the quasi-Fermi level of TiO_{2} particles, that is, their conduction band edge. In order to avoid scavenging of photogenerated electrons by oxygen dissolved in the solution, the electrolyte should be deaerated by purging with an inert gas prior to the measurement. Figure 7(c) shows a typical photovoltammogram recorded under interrupted illumination on a dense compact TiO_{2} electrode during the cathodic sweep. It should be noted that the absolute values of obtained are sometimes anodically shifted since the recombination becomes practically complete already at potentials relatively far (0.1–0.3 V) from the conduction band edge. Nevertheless, this method provides valuable information on shifts of , particularly when a direct comparison can be drawn from measurements on different samples under otherwise identical conditions.

##### 3.3. Open-Circuit Photovoltage Measurements

Apart from the capacitance measurements and the photocurrent onset determination, the value of can be also determined from the dependence of the electrode open-circuit potential () on the illumination intensity (Figure 8). Under open-circuit conditions, the photogenerated holes can accumulate at the surface, which with increasing light intensity lowers the barrier (see Figure 3) for electrons until the electrons can reach the surface at the same rate as holes. At the same time, the quasi-Fermi level (measured as ) rises because of the higher occupancy of the conduction band. Accordingly, at sufficiently high-intensity, becomes constant and this value is very close to the potential of the conduction band edge [80, 125, 185–187]. In order to avoid reaction of photogenerated electrons with oxygen in the electrolyte, which would decrease the photovoltage, it is necessary to purge the solution with inert gas.

Figures 9(a), 9(b), and 9(c) show versus relative light intensity plots measured for a compact TiO_{2} film at different pH values. It is seen that becomes independent of intensity when the latter exceeds relative values of 90%. The values plotted in Figure 9(d) show a nearly Nernstian linear dependence on pH with V versus NHE, in agreement with values reported for anatase TiO_{2} [172]. Interestingly, the open-circuit photovoltage method yields reliable results also in case of nanocrystalline photoelectrodes [188, 189]. Under high-intensity illumination, the electrons accumulating in the conduction band and traps right bellow the conduction band edge cause the Fermi level of the conductive glass substrate to shift to the vicinity of of TiO_{2}. It is again emphasized that intense purging with inert gas is absolutely necessary in order to avoid scavenging of photogenerated electrons by oxygen dissolved in solution.

##### 3.4. Spectroelectrochemical Measurements on Transparent Films

The fact that many nanocrystalline films are *transparent* offers the possibility to determine the position of the conduction band edges using the spectroelectrochemical method of Fitzmaurice et al. [190–192]. The principle of this method is schematically depicted in Figure 10. The Fermi level of ITO, (ITO), can be controlled by applied potential, whereas the position of the conduction band edge of the transparent nanocrystalline TiO_{2}, (TiO_{2}), depends only on the pH of the solution. At a constant pH, applying potentials more negative than (TiO_{2}) leads to injection of electrons from ITO into the conduction band of TiO_{2} (Figure 10(b)). During injection of electrons into the conduction band, the TiO_{2} nanoparticles are not at thermodynamic equilibrium anymore; the Fermi level of TiO_{2} is therefore properly designated as a *quasi*-Fermi level, , and practically merges with the conduction band edge, . The occupation of states near the conduction band edge results in a shift to higher energies of the bandgap absorption edge (i.e., in Figures 10(a) and 10(b))—the so-called Burstein-Moss shift [193, 194]. From the spectroscopic point of view, this has two consequences. First, at potentials more negative than (TiO_{2}), the difference in absorbance at wavelengths lower than the typical absorption band edge (e.g., at 350 nm) becomes negative. Second, the absorbance at 780 nm increases due to the intraband transitions of free electrons in the conduction band (Figure 10(c)) [190, 191, 195].

In this context, it should be noted that the nanocrystalline TiO_{2} has often a high density of electron traps that are distributed exponentially in the bandgap below the conduction band edge [196–200]. These traps can be obviously filled at potentials slightly more positive than and can also contribute to absorbance changes. This means that in practice it might be difficult to discern where exactly the rise in absorbance coincides with the potential of the conduction band edge. Figure 11(a) shows the absorbance changes at of a transparent nanocrystalline TiO_{2} film at two different pH values. The potentials of were in this case, somewhat arbitrarily, read off at points where the absorbance change was approximately 0.005. The values (which coincide with the values) plotted in Figure 11(b) show a nearly Nernstian linear dependence on pH with V versus NHE.

##### 3.5. Quasi-Fermi Level Measurements on TiO_{2} Powder Suspensions

In the field of heterogeneous photocatalysis, TiO_{2}-based materials are often employed in the form of nanocrystalline powders. The quasi-Fermi level of electrons, , can be in case of powder suspensions determined by the method of Roy et al. [29, 201] that draws on a similar method introduced previously by Bard et al. [202–204] In Roy’s method, the pH dependence of the potential of a platinum electrode immersed in an irradiated suspension of a semiconductor powder (Figure 12) is recorded in the presence of an electron acceptor with pH-independent reduction potential. As an electron acceptor, (methyl viologen; 1,1′-dimethyl-4,4′-bipyridinium dichloride; V versus NHE) [130] is typically used (Figure 12(b)).

The principle of the method is depicted in Figure 13. At the beginning of the measurement, the pH of the solution is very low and the electrons generated in the conduction band do not have enough reducing power to reduce (Figure 13(a)). Upon increasing the pH of the solution, the band edges of TiO_{2} shift to more negative potentials (see above Section 2.2), which makes at some point the electron transfer to in the electrolyte possible (Figure 13(b)). The platinum electrode serves as a simple redox electrode in this case, and its potential shifts more negative with the increasing concentration of the reduced form of methyl viologen () in the solution. The inflection point (pH_{0}) of the potential-pH curve (Figure 12(c)) determines the pH value at which coincides with . Assuming Nernstian shift of band edges (0.059 V/pH unit) [125],
Using this procedure, at pH = 7 of anatase TiO_{2} powder (Hombikat UV 100) was determined as V versus NHE, which is in a very good agreement with reported values for single-crystal anatase (−0.58 V versus NHE) [172]. It should be also noted that efficient scavenging of photogenerated holes is essential during these measurements. In some cases—on doped or surface-modified TiO_{2} samples, for example—an additional hole scavenger must be added in order to avoid severe recombination. Such a scavenger should be very easily oxidizable (e.g., iodide), and at the same time it should not produce strongly reducing radicals upon one-hole oxidation (e.g., ethanol, isopropanol) since these are also able to reduce , which would falsify the resulting values of [205].

#### 4. Conclusions

TiO_{2} nanomaterials play a key role in the development of various kinds of photochemical systems and devices, particularly in the field of heterogeneous photocatalysis and photoelectrochemistry. In the last years, we have witnessed a real boom of diverse strategies for fabrication of new types of TiO_{2}-based materials showing an extreme variety in terms of composition, morphology, and surface properties. Although the knowledge of the position of the band edges on the potential scale is a crucial prerequisite for understanding the photoactivity of the system and for further optimization of its performance, it has been in recent years typically only rarely directly experimentally addressed. In this paper it has been shown that in case of TiO_{2} the general strategy for band edges determination usually consists in the measurement of the flatband potential and/or the quasi-Fermi level of electrons. Apart from “classical” approaches (capacitance measurements) developed in the field of semiconductor physics for well-defined samples in the form of single crystals, several novel techniques have been developed recently. These are particularly important since they are also suitable for measurements on non-ideal nanostructured, porous, and particulate materials, which represent the majority of currently newly developed materials. The methods discussed above included elaborate photoelectrochemical and spectroelectrochemical methods applicable on compact and nanocrystalline thin films, as well as on powder suspensions. Obviously, in case of many systems, a combination of several methods will give a more solid and complete assessment of the energetics at the solid/solution interface. It is hoped that this paper will serve as a useful resource for many scientists working in the field of photoactive nanomaterials and as an impetus for the development of further methods that will allow for better understanding and improvement of the photoactivity of photochemical systems and devices.

#### Acknowledgments

The financial support by the MIWFT-NRW within the project “Anorganische Nanomaterialien für Anwendungen in der Photokatalyse: Wasseraufbereitung und Wasserstoff-gewinnung” and the support by the Center for Electrochemical Sciences (CES) are gratefully acknowledged. The company Sachtleben Chemie is acknowledged for providing a free sample of Hombikat UV 100.

#### References

- C. Renz, “Photo-reactions of the oxides of titanium, cerium, and the earth-acids,”
*Helvetica Chimica Acta*, vol. 4, pp. 961–968, 1921. View at Google Scholar - G. G. Rao and N. R. Dhar, “Photosensitized oxidation of ammonia and ammonium salts and the problem of nitrification in soils,”
*Soil Science*, vol. 31, pp. 379–384, 1931. View at Google Scholar - N. R. Dhar and S. K. Mukherjee, “Photosynthesis of amino acids in vitro,”
*Nature*, vol. 134, no. 3387, p. 499, 1934. View at Google Scholar · View at Scopus - A. A. Krasnovskii and V. S. Kiselev, “A method for testing the activity of titanium dioxide in paint films,”
*Tekh. Okraski*, no. 3, pp. 26–27, 1940. View at Google Scholar - C. F. Goodeve and J. A. Kitchener, “Photosensitisation by titanium dioxide,”
*Transactions of the Faraday Society*, vol. 34, pp. 570–579, 1938. View at Publisher · View at Google Scholar · View at Scopus - A. E. Jacobsen, “Titanium dioxide pigments. Correlation between photochemical reactivity and chalking,”
*Journal of Industrial and Engineering Chemistry*, vol. 41, pp. 523–526, 1949. View at Google Scholar - A. A. Krasnovskii and T. N. Gurevich, “Relation between atmospheric stability of pigmented paint films and the pigment-photosensitized formation of peroxide compounds,,”
*Doklady Akademii Nauk SSSR*, vol. 74, pp. 569–572, 1950. View at Google Scholar - A. A. Krasnovskii and T. N. Gurevich, “Photocatalytic action of some metal oxides,”
*Doklady Akademii Nauk SSSR*, vol. 75, pp. 715–718, 1950. View at Google Scholar - A. Fujishima and K. Honda, “Photosensitive electrode reactions. III. Electrochemical evidence for the mechanism of the primary stage of photosynthesis,”
*Bulletin of the Chemical Society of Japan*, vol. 44, no. 4, pp. 1148–1150, 1971. View at Google Scholar - A. Fujishima and K. Honda, “Electrochemical photolysis of water at a semiconductor electrode,”
*Nature*, vol. 238, no. 5358, pp. 37–38, 1972. View at Publisher · View at Google Scholar · View at Scopus - A. Fujishima, K. Honda, and S. Kikuchi, “Photochemical reactions of semiconductors. I. Photosensitized electrolytic oxidation on semiconducting n-type TiO
_{2}electrode,”*Kogyo Kagaku Zasshi*, vol. 72, no. 1, pp. 108–113, 1969. View at Google Scholar - M. S. Wrighton, P. T. Wolczanski, and A. B. Ellis, “Photoelectrolysis of water by irradiation of platinized n-type semiconducting metal oxides,”
*Journal of Solid State Chemistry*, vol. 22, no. 1, pp. 17–29, 1977. View at Google Scholar · View at Scopus - M. Sharon and S. Licht, “Solar photoelectrochemical generation of hydrogen fuel,” in
*Encyclopedia of Electrochemistry*, S. Licht, Ed., vol. 6, pp. 346–357, Wiley-VCH, Weinheim, Germany, 2003. View at Google Scholar - K. Rajeshwar, “Hydrogen generation at irradiated oxide semiconductor-solution interfaces,”
*Journal of Applied Electrochemistry*, vol. 37, no. 7, pp. 765–787, 2007. View at Publisher · View at Google Scholar · View at Scopus - X. Chen, S. Shen, L. Guo, and S. S. Mao, “Semiconductor-based photocatalytic hydrogen generation,”
*Chemical Reviews*, vol. 110, no. 11, pp. 6503–6570, 2010. View at Publisher · View at Google Scholar · View at PubMed · View at Scopus - Z. Chen, T. F. Jaramillo, T. G. Deutsch et al., “Accelerating materials development for photoelectrochemical hydrogen production: standards for methods, definitions, and reporting protocols,”
*Journal of Materials Research*, vol. 25, no. 1, pp. 3–16, 2010. View at Publisher · View at Google Scholar · View at Scopus - M. R. Hoffmann, S. T. Martin, W. Choi, and D. W. Bahnemann, “Environmental applications of semiconductor photocatalysis,”
*Chemical Reviews*, vol. 95, no. 1, pp. 69–96, 1995. View at Google Scholar · View at Scopus - A. Fujishima, T. N. Rao, and D. A. Tryk, “Titanium dioxide photocatalysis,”
*Journal of Photochemistry and Photobiology C*, vol. 1, no. 1, pp. 1–21, 2000. View at Google Scholar · View at Scopus - D. A. Tryk, A. Fujishima, and K. Honda, “Recent topics in photoelectrochemistry: achievements and future prospects,”
*Electrochimica Acta*, vol. 45, no. 15-16, pp. 2363–2376, 2000. View at Google Scholar · View at Scopus - O. Carp, C. L. Huisman, and A. Reller, “Photoinduced reactivity of titanium dioxide,”
*Progress in Solid State Chemistry*, vol. 32, no. 1-2, pp. 33–177, 2004. View at Publisher · View at Google Scholar · View at Scopus - A. L. Linsebigler, G. Lu, and J. T. Yates Jr., “Photocatalysis on TiO
_{2}surfaces: principles, mechanisms, and selected results,”*Chemical Reviews*, vol. 95, no. 3, pp. 735–758, 1995. View at Google Scholar - T. L. Thompson and J. T. Yates Jr., “TiO
_{2}-based photocatalysis: surface defects, oxygen and charge transfer,”*Topics in Catalysis*, vol. 35, no. 3-4, pp. 197–210, 2005. View at Publisher · View at Google Scholar - A. Fujishima, X. Zhang, and D. A. Tryk, “TiO
_{2}photocatalysis and related surface phenomena,”*Surface Science Reports*, vol. 63, no. 12, pp. 515–582, 2008. View at Publisher · View at Google Scholar - B. Ohtani, “Preparing articles on photocatalysis—beyond the illusions, misconceptions, and speculation,”
*Chemistry Letters*, vol. 37, no. 3, pp. 217–229, 2008. View at Google Scholar · View at Scopus - B. Ohtani, “Photocatalysis A to Z-What we know and what we do not know in a scientific sense,”
*Journal of Photochemistry and Photobiology C*, vol. 11, no. 4, pp. 157–178, 2011. View at Publisher · View at Google Scholar · View at Scopus - S. N. Frank and A. J. Bard, “Heterogeneous photocatalytic oxidation of cyanide ion in aqueous solutions at TiO
_{2}powder,”*Journal of the American Chemical Society*, vol. 99, no. 1, pp. 303–304, 1977. View at Google Scholar - S. N. Frank and A. J. Bard, “Heterogeneous photocatalytic oxidation of cyanide and sulfite in aqueous solutions at semiconductor powders,”
*Journal of Physical Chemistry*, vol. 81, no. 15, pp. 1484–1488, 1977. View at Google Scholar · View at Scopus - S. Sakthivel, M. Janczarek, and H. Kisch, “Visible light activity and photoelectrochemical properties of nitrogen-doped TiO
_{2},”*Journal of Physical Chemistry B*, vol. 108, no. 50, pp. 19384–19387, 2004. View at Publisher · View at Google Scholar · View at Scopus - H. Kisch, G. Burgeth, and W. Macyk, “Visible light photocatalysis by a titania transition metal complex,”
*Advances in Inorganic Chemistry*, vol. 56, pp. 241–259, 2004. View at Publisher · View at Google Scholar · View at Scopus - S. Sakthivel and H. Kisch, “Daylight photocatalysis by carbon-modified titanium dioxide,”
*Angewandte Chemie—International Edition*, vol. 42, no. 40, pp. 4908–4911, 2003. View at Publisher · View at Google Scholar · View at PubMed · View at Scopus - S. Sakthivel and H. Kisch, “Photocatalytic and photoelectrochemical properties of nitrogen-doped titanium dioxide,”
*ChemPhysChem*, vol. 4, no. 5, pp. 487–490, 2003. View at Publisher · View at Google Scholar · View at PubMed · View at Scopus - W. Macyk, G. Burgeth, and H. Kisch, “Photoelectrochemical properties of platinum(IV) chloride surface modified TiO
_{2},”*Photochemical and Photobiological Sciences*, vol. 2, no. 3, pp. 322–328, 2003. View at Publisher · View at Google Scholar · View at Scopus - G. Burgeth and H. Kisch, “Photocatalytic and photoelectrochemical properties ot titaniachloroplatinate(IV),”
*Coordination Chemistry Reviews*, vol. 230, no. 1-2, pp. 41–47, 2002. View at Google Scholar · View at Scopus - H. Kisch and W. Macyk, “Visible-light photocatalysis by modified titania,”
*ChemPhysChem*, vol. 3, no. 5, pp. 399–400, 2002. View at Publisher · View at Google Scholar - C. Lettmann, K. Hildenbrand, H. Kisch, W. Macyk, and W. F. Maier, “Visible light photodegradation of 4-chlorophenol with a coke-containing titanium dioxide photocatalyst,”
*Applied Catalysis B*, vol. 32, no. 4, pp. 215–227, 2001. View at Publisher · View at Google Scholar · View at Scopus - W. Macyk and H. Kisch, “Photosensitization of crystalline and amorphous titanium dioxide by platinum(IV) chloride surface complexes,”
*Chemistry*, vol. 7, no. 9, pp. 1862–1867, 2001. View at Publisher · View at Google Scholar - C. Chen, W. Ma, and J. Zhao, “Semiconductor-mediated photodegradation of pollutants under visible-light irradiation,”
*Chemical Society Reviews*, vol. 39, no. 11, pp. 4206–4219, 2010. View at Publisher · View at Google Scholar · View at PubMed · View at Scopus - D. Mitoraj, R. Beránek, and H. Kisch, “Mechanism of aerobic visible light formic acid oxidation catalyzed by poly(tri-s-triazine) modified titania,”
*Photochemical and Photobiological Sciences*, vol. 9, no. 1, pp. 31–38, 2010. View at Publisher · View at Google Scholar · View at PubMed · View at Scopus - D. Mitoraj and H. Kisch, “On the mechanism of urea-induced titania modification,”
*Chemistry*, vol. 16, no. 1, pp. 261–269, 2010. View at Publisher · View at Google Scholar · View at PubMed · View at Scopus - R. Wang, K. Hashimoto, A. Fujishima et al., “Light-induced amphiphilic surfaces,”
*Nature*, vol. 388, no. 6641, pp. 431–432, 1997. View at Publisher · View at Google Scholar · View at Scopus - R. Wang, K. Hashimoto, A. Fujishima et al., “Photogeneration of highly amphiphilic TiO
_{2},”*Advanced Materials*, vol. 10, no. 2, pp. 135–138, 1998. View at Google Scholar · View at Scopus - R. Wang, N. Sakai, A. Fujishima, T. Watanabe, and K. Hashimoto, “Studies of surface wettability conversion on TiO
_{2},”*Journal of Physical Chemistry B*, vol. 103, no. 12, pp. 2188–2194, 1999. View at Google Scholar · View at Scopus - T. Zubkoy, D. Stahl, T. L. Thompson, D. Panayotov, O. Diwald, and J. T. Yates Jr., “Ultraviolet light-induced hydrophilicity effect on TiO
_{2}(110) ($1\times 1$). Dominant role of the photooxidation of adsorbed hydrocarbons causing wetting by water droplets,”*Journal of Physical Chemistry B*, vol. 109, no. 32, pp. 15454–15462, 2005. View at Publisher · View at Google Scholar · View at PubMed - B. Kraeutler and A. J. Bard, “Heterogeneous photocatalytic synthesis of methane from acetic acid—new Kolbe reaction pathway,”
*Journal of the American Chemical Society*, vol. 100, no. 7, pp. 2239–2240, 1978. View at Google Scholar · View at Scopus - P. Du, J. A. Moulijn, and G. Mul, “Selective photo(catalytic)-oxidation of cyclohexane: effect of wavelength and TiO
_{2}structure on product yields,”*Journal of Catalysis*, vol. 238, no. 2, pp. 342–352, 2006. View at Publisher · View at Google Scholar - F. Parrino, A. Ramakrishnan, and H. Kisch, “Semiconductor-photocatalyzed sulfoxidation of alkanes,”
*Angewandte Chemie—International Edition*, vol. 47, no. 37, pp. 7107–7109, 2008. View at Publisher · View at Google Scholar · View at PubMed · View at Scopus - Q. Wang, M. Zhang, C. Chen, W. Ma, and J. Zhao, “Photocatalytic aerobic oxidation of alcohols on TiO
_{2},”*Angewandte Chemie—International Edition*, vol. 49, no. 43, pp. 7976–7979, 2010. View at Publisher · View at Google Scholar · View at PubMed · View at Scopus - S. I. Naya, A. Inoue, and H. Tada, “Self-assembled heterosupramolecular visible light photocatalyst consisting of gold nanoparticle-loaded titanium(IV) dioxide and surfactant,”
*Journal of the American Chemical Society*, vol. 132, no. 18, pp. 6292–6293, 2010. View at Publisher · View at Google Scholar · View at PubMed · View at Scopus - X. Lang, H. Ji, C. Chen, W. Ma, and J. Zhao, “Selective formation of imines by aerobic photocatalytic oxidation of amines on TiO
_{2},”*Angewandte Chemie—International Edition*, vol. 50, no. 17, pp. 3934–3937, 2011. View at Publisher · View at Google Scholar · View at PubMed - H. Sakai, R. Baba, K. Hashimoto, Y. Kubota, and A. Fujishima, “Selective killing of a single cancerous T24 cell with TiO
_{2}semiconducting microelectrode under irradiation,”*Chemistry Letters*, no. 3, pp. 185–186, 1995. View at Google Scholar - A. H. Sakai, R. X. Cai, T. Yoshioka, Y. Kubota, K. Hashimoto, and A. Fujishima, “Intracellular Ca
^{2+}concentration change of T24 cell under irradiation in the presence of TiO_{2}ultrafine particles,”*Biochimica et Biophysica Acta*, vol. 1201, no. 2, pp. 259–265, 1994. View at Publisher · View at Google Scholar - R. Cai, Y. Kubota, T. Shuin, H. Sakai, K. Hashimoto, and A. Fujishima, “Induction of cytotoxicity by photoexcited TiO2 particles,”
*Cancer Research*, vol. 52, no. 8, pp. 2346–2348, 1992. View at Google Scholar - R. Cai, K. Hashimoto, Y. Kubota, and A. Fujishima, “Increment of photocatalytic killing of cancer cells using titanium dioxide with the aid of superoxide dismutase,”
*Chemistry Letters*, no. 3, pp. 427–430, 1992. View at Google Scholar - R. Cai, K. Hashimoto, K. Itoh, Y. Kubota, and A. Fujishima, “Photokilling of malignant cells with ultrafine TiO
_{2}powder,”*Bulletin of the Chemical Society of Japan*, vol. 64, no. 4, pp. 1268–1273, 1991. View at Google Scholar - H. Gerischer and H. Tributsch, “Electrochemical studies on the spectral sensitization of zinc oxide single crystals,”
*Berichte der Bunsen-Gesellschaft*, vol. 72, no. 3, pp. 437–445, 1968. View at Google Scholar - H. Tributsch and H. Gerischer, “Electrochemical studies on the mechanism of sensitization and supersensitization of zinc oxide single crystals,”
*Berichte der Bunsen-Gesellschaft*, vol. 73, no. 3, pp. 251–260, 1969. View at Google Scholar - H. Tributsch and H. Gerischer, “Use of semiconductor electrodes in the study of photochemical reactions,”
*Berichte der Bunsen-Gesellschaft*, vol. 73, no. 8-9, pp. 850–854, 1969. View at Google Scholar - H. Tributsch, “Reaction of excited chlorophyll molecules at electrodes and in photosynthesis,”
*Photochemistry and Photobiology*, vol. 16, no. 4, pp. 261–269, 1972. View at Google Scholar - H. Tributsch and M. Calvin, “Electrochemistry of excited molecules. Photoelectrochemical reactions of chlorophylls,”
*Photochemistry and Photobiology*, vol. 14, no. 2, pp. 95–112, 1971. View at Google Scholar - M. Matsumura, S. Matsudaira, H. Tsubomura, M. Takata, and H. Yanagida, “Dye sensitization and surface structures of semiconductor electrodes,”
*Industrial & Engineering Chemistry Product Research and Development*, vol. 19, no. 3, pp. 415–421, 1980. View at Google Scholar · View at Scopus - J. Desilvestro, M. Grätzel, L. Kavan, J. Moser, and J. Augustynski, “Highly efficient sensitization of titanium dioxide,”
*Journal of the American Chemical Society*, vol. 107, no. 10, pp. 2988–2990, 1985. View at Google Scholar · View at Scopus - B. O'Regan and M. Grätzel, “A low-cost, high-efficiency solar cell based on dye-sensitized colloidal TiO
_{2}films,”*Nature*, vol. 353, no. 6346, pp. 737–740, 1991. View at Google Scholar - M. Grätzel, “Photoelectrochemical cells,”
*Nature*, vol. 414, no. 6861, pp. 338–344, 2001. View at Publisher · View at Google Scholar · View at PubMed · View at Scopus - B. C. O'Regan and J. R. Durrant, “Kinetic and energetic paradigms for dyesensitized solar cells: moving from the ideal to the real,”
*Accounts of Chemical Research*, vol. 42, no. 11, pp. 1799–1808, 2009. View at Publisher · View at Google Scholar · View at PubMed · View at Scopus - L. Spanhel, H. Weller, and A. Henglein, “Photochemistry of semiconductor colloids. 22. Electron injection from illuminated CdS into attached TiO
_{2}and ZnO particles,”*Journal of the American Chemical Society*, vol. 109, no. 22, pp. 6632–6635, 1987. View at Google Scholar - R. Vogel, P. Hoyer, and H. Weller, “Quantum-sized PbS, CdS, Ag
_{2}S, Sb_{2}S_{3}, and Bi_{2}S_{3}particles as sensitizers for various nanoporous wide-bandgap semiconductors,”*Journal of Physical Chemistry*, vol. 98, no. 12, pp. 3183–3188, 1994. View at Google Scholar - A. J. Nozik, “Quantum dot solar cells,”
*Physica E*, vol. 14, no. 1-2, pp. 115–120, 2002. View at Publisher · View at Google Scholar · View at Scopus - L. M. Peter, D. J. Riley, E. J. Tull, and K. G.U. Wijayantha, “Photosensitization of nanocrystalline TiO
_{2}by self-assembled layers of CdS quantum dots,”*Chemical Communications*, no. 10, pp. 1030–1031, 2002. View at Google Scholar - P. V. Kamat, “Quantum dot solar cells. Semiconductor nanocrystals as light harvesters,”
*Journal of Physical Chemistry C*, vol. 112, no. 48, pp. 18737–18753, 2008. View at Publisher · View at Google Scholar · View at Scopus - P. V. Kamat, K. Tvrdy, D. R. Baker, and J. G. Radich, “Beyond photovoltaics: semiconductor nanoarchitectures for liquid-junction solar cells,”
*Chemical Reviews*, vol. 110, no. 11, pp. 6664–6688, 2010. View at Publisher · View at Google Scholar · View at PubMed · View at Scopus - Y. Tian and T. Tatsuma, “Mechanisms and applications of plasmon-induced charge separation at TiO
_{2}films loaded with gold nanoparticles,”*Journal of the American Chemical Society*, vol. 127, no. 20, pp. 7632–7637, 2005. View at Publisher · View at Google Scholar · View at PubMed - Z. Liu, W. Hou, P. Pavaskar, M. Aykol, and S. B. Cronin, “Plasmon resonant enhancement of photocatalytic water splitting under visible illumination,”
*Nano Letters*, vol. 11, no. 3, pp. 1111–1116, 2011. View at Publisher · View at Google Scholar · View at PubMed · View at Scopus - J. Tang, “Interaction between noble metal nanoparticles and light for contaminant decomposition,”
*ChemSusChem*, vol. 3, no. 7, pp. 800–801, 2010. View at Publisher · View at Google Scholar · View at PubMed · View at Scopus - Y. Nishijima, K. Ueno, Y. Yokota, K. Murakoshi, and H. Misawa, “Plasmon-assisted photocurrent generation from visible to near-infrared wavelength using a Au-nanorods/TiO
_{2},”*Journal of Physical Chemistry Letters*, vol. 1, no. 13, pp. 2031–2036, 2010. View at Publisher · View at Google Scholar · View at Scopus - S. I. Naya, A. Inoue, and H. Tada, “Visible-light activity enhancement of gold-nanoparticle-loaded titanium(IV) dioxide by preferential excitation of localized surface plasmon resonance,”
*ChemPhysChem*, vol. 12, no. 15, pp. 2719–2723, 2011. View at Publisher · View at Google Scholar · View at PubMed - H. Kisch, L. Zang, C. Lange, W. F. Maier, C. Antonius, and D. Meissner, “Modified, amorphous titania—a hybrid semiconductor for detoxification and current generation by visible light,”
*Angewandte Chemie—International Edition*, vol. 37, no. 21, pp. 3034–3036, 1998. View at Publisher · View at Google Scholar - E. Vrachnou, N. Vlachopoulos, and M. Grätzel, “Efficient visible light sensitization of TiO
_{2}a by surface complexation with $\text{Fe}{(\text{CN})}_{6}^{4-}$,”*Journal of the Chemical Society, Chemical Communications*, vol. 37, no. 12, pp. 868–870, 1987. View at Publisher · View at Google Scholar · View at Scopus - M. Khoudiakov, A. R. Parise, and B. S. Brunschwig, “Interfacial electron transfer in ${\text{Fe}}^{\text{II}}{(\text{CN})}_{6}^{4-}$ sensitized TiO
_{2}nanoparticles: a study of direct charge injection by electroabsorption spectroscopy,”*Journal of the American Chemical Society*, vol. 125, no. 15, pp. 4637–4642, 2003. View at Publisher · View at Google Scholar · View at PubMed - W. Macyk, G. Stochel, and K. Szaciłowski, “Photosensitization and the photocurrent switching effect in nanocrystalline titanium dioxide functionalized with Iron(II) complexes: a comparative study,”
*Chemistry*, vol. 13, no. 20, pp. 5676–5687, 2007. View at Publisher · View at Google Scholar · View at PubMed · View at Scopus - R. Beranek and H. Kisch, “Surface-modified anodic TiO
_{2}films for visible light photocurrent response,”*Electrochemistry Communications*, vol. 9, no. 4, pp. 761–766, 2007. View at Publisher · View at Google Scholar - R. Beranek and H. Kisch, “Tuning the optical and photoelectrochemical properties of surface-modified TiO
_{2},”*Photochemical and Photobiological Sciences*, vol. 7, no. 1, pp. 40–48, 2007. View at Publisher · View at Google Scholar · View at PubMed · View at Scopus - R. Beranek, J. M. Macak, M. Gärtner, K. Meyer, and P. Schmuki, “Enhanced visible light photocurrent generation at surface-modified TiO
_{2}nanotubes,”*Electrochimica Acta*, vol. 54, no. 9, pp. 2640–2646, 2009. View at Publisher · View at Google Scholar · View at Scopus - D. Mitoraj and H. Kisch, “The nature of nitrogen-modified titanium dioxide photocatalysts active in visible light,”
*Angewandte Chemie—International Edition*, vol. 47, no. 51, pp. 9975–9978, 2008. View at Publisher · View at Google Scholar · View at PubMed · View at Scopus - H. Irie, K. Kamiya, T. Shibanuma et al., “Visible light-sensitive Cu(II)-grafted TiO
_{2}photocatalysts: activities and X-ray absorption fine structure analyses,”*Journal of Physical Chemistry C*, vol. 113, no. 24, pp. 10761–10766, 2009. View at Publisher · View at Google Scholar - H. Yu, H. Irie, Y. Shimodaira et al., “An efficient visible-light-sensitive Fe(III)-grafted TiO
_{2}photocatalyst,”*Journal of Physical Chemistry C*, vol. 114, no. 39, pp. 16481–16487, 2010. View at Publisher · View at Google Scholar · View at Scopus - K. Palmisano, V. Augugliaro, A. Sclafani, and M. Schiavello, “Activity of chromium-ion-doped titania for the dinitrogen photoreduction to ammonia and for the phenol photodegradation,”
*Journal of Physical Chemistry*, vol. 92, no. 23, pp. 6710–6713, 1988. View at Google Scholar · View at Scopus - A. Di Paola, G. Marcì, L. Palmisano et al., “Preparation of polycrystalline TiO
_{2}photocatalysts impregnated with various transition metal ions: characterization and photocatalytic activity for the degradation of 4-nitrophenol,”*Journal of Physical Chemistry B*, vol. 106, no. 3, pp. 637–645, 2002. View at Publisher · View at Google Scholar - M. Anpo, “Use of visible light. Second-generation titanium oxide photocatalysts prepared by the application of an advanced metal ion-implantation method,”
*Pure and Applied Chemistry*, vol. 72, no. 9, pp. 1787–1792, 2000. View at Google Scholar · View at Scopus - S. U. M. Khan, M. Al-Shahry, and W. B. Ingler Jr., “Efficient photochemical water splitting by a chemically modified n-TiO
_{2},”*Science*, vol. 297, no. 5590, pp. 2243–2245, 2002. View at Publisher · View at Google Scholar · View at PubMed · View at Scopus - T. Hirai, I. Tari, and J. Yamaura, “Titanium nitride oxide (TiN0.07O1.93) semiconductor electrodes for photoassisted oxidation of water,”
*Bulletin of the Chemical Society of Japan*, vol. 51, no. 10, pp. 3057–3058, 1978. View at Google Scholar - S. Sato, “Photocatalytic activity of nitrogen oxide (NO
_{x})-doped titanium dioxide in the visible light region,”*Chemical Physics Letters*, vol. 123, no. 1-2, pp. 126–128, 1986. View at Google Scholar - R. Asahi, T. Morikawa, T. Ohwaki, K. Aoki, and Y. Taga, “Visible-light photocatalysis in nitrogen-doped titanium oxides,”
*Science*, vol. 293, no. 5528, pp. 269–271, 2001. View at Publisher · View at Google Scholar · View at PubMed · View at Scopus - A. Ghicov, J. M. Macak, H. Tsuchiya et al., “TiO
_{2}nanotube layers: dose effects during nitrogen doping by ion implantation,”*Chemical Physics Letters*, vol. 419, no. 4–6, pp. 426–429, 2006. View at Publisher · View at Google Scholar - T. Lindgren, J. M. Mwabora, E. Avandaño et al., “Photoelectrochemical and optical properties of nitrogen doped titanium dioxide films prepared by reactive DC magnetron sputtering,”
*Journal of Physical Chemistry B*, vol. 107, no. 24, pp. 5709–5716, 2003. View at Google Scholar · View at Scopus - H. Irie, Y. Watanabe, and K. Hashimoto, “Nitrogen-concentration dependence on photocatalytic activity of ${\text{TiO}}_{2-\text{x}}{\text{N}}_{\text{x}}$ powders,”
*Journal of Physical Chemistry B*, vol. 107, no. 23, pp. 5483–5486, 2003. View at Google Scholar · View at Scopus - C. Burda, Y. Lou, X. Chen, A. C. S. Samia, J. Stout, and J. L. Gole, “Enhanced nitrogen doping in TiO
_{2}Nanoparticles,”*Nano Letters*, vol. 3, no. 8, pp. 1049–1051, 2003. View at Publisher · View at Google Scholar · View at Scopus - M. Sathish, B. Viswanathan, R. P. Viswanath, and C. S. Gopinath, “Synthesis, characterization, electronic structure, and photocatalytic activity of nitrogen-doped TiO
_{2}nanocatalyst,”*Chemistry of Materials*, vol. 17, no. 25, pp. 6349–6353, 2005. View at Publisher · View at Google Scholar · View at Scopus - T. Umebayashi, T. Yamaki, H. Itoh, and K. Asai, “Band gap narrowing of titanium dioxide by sulfur doping,”
*Applied Physics Letters*, vol. 81, no. 3, p. 454, 2002. View at Publisher · View at Google Scholar · View at Scopus - T. Ohno, “Preparation of visible light active S-doped TiO
_{2}photocatalysts and their photocatalytic activities,”*Water Science and Technology*, vol. 49, no. 4, pp. 159–163, 2004. View at Google Scholar - M. Zheng, Y. Cui, X. Li, S. Liu, and Z. Tang, “Photoelectrochemical sensing of glucose based on quantum dot and enzyme nanocomposites,”
*Journal of Electroanalytical Chemistry*, vol. 656, no. 1-2, pp. 167–173, 2011. View at Publisher · View at Google Scholar - G. L. Wang, J. J. Xu, and H. Y. Chen, “Dopamine sensitized nanoporous TiO
_{2}film on electrodes: photoelectrochemical sensing of NADH under visible irradiation,”*Biosensors and Bioelectronics*, vol. 24, no. 8, pp. 2494–2498, 2009. View at Publisher · View at Google Scholar · View at PubMed - K. Szaciłowski and W. Macyk, “Chemical switches and logic gates based on surface modified semiconductors,”
*Comptes Rendus Chimie*, vol. 9, no. 2, pp. 315–324, 2006. View at Publisher · View at Google Scholar · View at Scopus - M. Hebda, G. Stochel, K. Szaciłowski, and W. Macyk, “Optoelectronic switches based on wide band gap semiconductors,”
*Journal of Physical Chemistry B*, vol. 110, no. 31, pp. 15275–15283, 2006. View at Publisher · View at Google Scholar · View at PubMed · View at Scopus - K. Szaciłowski, W. Macyk, and G. Stochel, “Light-driven OR and XOR programmable chemical logic gates,”
*Journal of the American Chemical Society*, vol. 128, no. 14, pp. 4550–4551, 2006. View at Publisher · View at Google Scholar · View at PubMed · View at Scopus - L. F. O. Furtado, A. D. P. Alexiou, L. Gonçalves, H. E. Toma, and K. Araki, “TiO
_{2}-based light-driven XOR/INH logic gates,”*Angewandte Chemie—International Edition*, vol. 45, no. 19, pp. 3143–3146, 2006. View at Publisher · View at Google Scholar · View at PubMed - R. Beranek and H. Kisch, “A hybrid semiconductor electrode for wavelength-controlled switching of the photocurrent direction,”
*Angewandte Chemie—International Edition*, vol. 47, no. 7, pp. 1320–1322, 2008. View at Publisher · View at Google Scholar · View at PubMed · View at Scopus - H. Ming, Z. Ma, H. Huang et al., “Nanoporous TiO
_{2}spheres with narrow pore size distribution and improved visible light photocatalytic abilities,”*Chemical Communications*, vol. 47, no. 28, pp. 8025–8027, 2011. View at Publisher · View at Google Scholar · View at PubMed - P. Roy, S. Berger, and P. Schmuki, “TiO
_{2}nanotubes: synthesis and applications,”*Angewandte Chemie—International Edition*, vol. 50, no. 13, pp. 2904–2939, 2011. View at Publisher · View at Google Scholar · View at PubMed - C. A. Grimes and G. K. Mor,
*TiO*, Springer, New York, NY, USA, 2009._{2}Nanotube Arrays: Synthesis, Properties, and Applications - W. P. Liao and J. J. Wu, “Wet chemical route to hierarchical TiO
_{2}nanodendrite/ nanoparticle composite anodes for dye-sensitized solar cells,”*Journal of Materials Chemistry*, vol. 21, no. 25, pp. 9255–9262, 2011. View at Publisher · View at Google Scholar - D. Fattakhova-Rohlfing, M. Wark, T. Brezesinski, B. M. Smarsly, and J. Rathouský, “Highly organized mesoporous TiO
_{2}films with controlled crystallinity: a Li-insertion study,”*Advanced Functional Materials*, vol. 17, no. 1, pp. 123–132, 2007. View at Publisher · View at Google Scholar - J. M. Szeifert, D. Fattakhova-Rohlfing, D. Georgiadou et al., “Brick and mortar strategy for the formation of highly crystalline mesoporous titania films from nanocrystalline building blocks,”
*Chemistry of Materials*, vol. 21, no. 7, pp. 1260–1265, 2009. View at Publisher · View at Google Scholar - J. Pan, G. Liu, G. Q. Lu, and H. M. Cheng, “On the true photoreactivity order of
$\{001\},\{010\}$, and $\{101\}$ facets of anatase TiO
_{2}crystals,”*Angewandte Chemie—International Edition*, vol. 50, no. 9, pp. 2133–2137, 2011. View at Publisher · View at Google Scholar · View at PubMed · View at Scopus - H. G. Yang, C. H. Sun, S. Z. Qiao et al., “Anatase TiO
_{2}single crystals with a large percentage of reactive facets,”*Nature*, vol. 453, no. 7195, pp. 638–641, 2008. View at Publisher · View at Google Scholar · View at PubMed - J. I. L. Chen, E. Loso, N. Ebrahim, and G. A. Ozin, “Synergy of slow photon and chemically amplified photochemistry in platinum nanocluster-loaded inverse titania opals,”
*Journal of the American Chemical Society*, vol. 130, no. 16, pp. 5420–5421, 2008. View at Publisher · View at Google Scholar · View at PubMed · View at Scopus - J. I. L. Chen, G. Von Freymann, S. Y. Choi, V. Kitaev, and G. A. Ozin, “Amplified photochemistry with slow photons,”
*Advanced Materials*, vol. 18, no. 14, pp. 1915–1919, 2006. View at Publisher · View at Google Scholar · View at Scopus - F. Sordello, C. Duca, V. Maurino, and C. Minero, “Photocatalytic metamaterials: TiO
_{2}inverse opals,”*Chemical Communications*, vol. 47, no. 21, pp. 6147–6149, 2011. View at Publisher · View at Google Scholar · View at PubMed - I. Bannat, K. Wessels, T. Oekermann, J. Rathousky, D. Bahnemann, and M. Wark, “Improving the photocatalytic performance of mesoporous titania films by modification with gold nanostructures,”
*Chemistry of Materials*, vol. 21, no. 8, pp. 1645–1653, 2009. View at Publisher · View at Google Scholar · View at Scopus - Q. Xiang, J. Yu, and M. Jaroniec, “Graphene-based semiconductor photocatalysts,”
*Chemical Society Reviews*, vol. 41, no. 2, pp. 782–796, 2012. View at Google Scholar - I. V. Lightcap, T. H. Kosel, and P. V. Kamat, “Anchoring semiconductor and metal nanoparticles on a two-dimensional catalyst mat. storing and shuttling electrons with reduced graphene oxide,”
*Nano Letters*, vol. 10, no. 2, pp. 577–583, 2010. View at Publisher · View at Google Scholar · View at PubMed · View at Scopus - W. Fan, Q. Lai, Q. Zhang, and Y. Wang, “Nanocomposites of TiO
_{2}and reduced graphene oxide as efficient photocatalysts for hydrogen evolution,”*Journal of Physical Chemistry C*, vol. 115, no. 21, pp. 10694–10701, 2011. View at Publisher · View at Google Scholar - M. D. Archer and A. J. Nozik, Eds.,
*Nanostructured and Photoelectrochemical Systems for Solar Photon Conversion*, Imperial College Press, 2008. - S. Trasatti, “The absolute electrode potential: an explanatory note. Recommendations 1986,”
*Pure and Applied Chemistry*, vol. 58, no. 7, pp. 955–966, 1986. View at Google Scholar · View at Scopus - V. Tripkovic, M. E. Björketun, E. Skúlason, and J. Rossmeisl, “Standard hydrogen electrode and potential of zero charge in density functional calculations,”
*Physical Review B*, vol. 84, no. 11, Article ID 115452, 2011. View at Publisher · View at Google Scholar - S. R. Morrison,
*Electrochemistry at Semiconductor and Oxidized Metal Electrodes*, Plenum Press, New York, NY, USA, 1980. - Y. V. Pleskov and Y. Y. Gurevich,
*Semiconductor Photoelectrochemistry*, Plenum Press, New York, NY, USA, 1986. - M. X. Tan, P. E. Laibinis, S. T. Nguyen, J. M. Kesselman, C. E. Stanton, and N. S. Lewis, “Principles and applications of semiconductor photoelectrochemistry,”
*Progress in Inorganic Chemistry*, vol. 41, pp. 21–144, 1994. View at Google Scholar - R. Memming,
*Semiconductor Electrochemistry*, Wiley-VCH, Weinheim, Germany, 2001. - K. Rajeshwar, “Fundamentals of semiconductor electrochemistry and photoelectrochemistry,” in
*Semiconductor Electrodes and Photoelectrochemistry*, S. Licht, Ed., vol. 6, pp. 1–57, Wiley-VCH, Weinheim, Germany, 2003. View at Google Scholar - P. Wardman, “Reduction potentials of one-electron couples involving free radicals in aqueous solution,”
*Journal of Physical and Chemical Reference Data*, vol. 18, no. 4, pp. 1637–1755, 1989. View at Google Scholar - R. B. Cundall, R. Rudham, and M. S. Salim, “Photocatalytic oxidation of propan-2-ol in the liquid phase by rutile,”
*Journal of the Chemical Society, Faraday Transactions 1*, vol. 72, pp. 1642–1651, 1976. View at Publisher · View at Google Scholar · View at Scopus - D. T. Sawyer and M. J. Gibian, “The chemistry of superoxide ion,”
*Tetrahedron*, vol. 35, no. 12, pp. 1471–1481, 1979. View at Google Scholar · View at Scopus - K. Okamoto, Y. Yamamoto, H. Tanaka, M. Tanaka, and A. Itaya, “Heterogeneous photocatalytic decomposition of phenol over anatase powder,”
*Bulletin of the Chemical Society of Japan*, vol. 58, no. 7, pp. 2015–2022, 1985. View at Google Scholar - H. Gerischer and A. Heller, “The role of oxygen in photooxidation of organic molecules on semiconductor particles,”
*Journal of Physical Chemistry*, vol. 95, no. 13, pp. 5261–5267, 1991. View at Google Scholar · View at Scopus - C. Creutz, B. S. Brunschwig, and N. Sutin, “Interfacial charge-transfer absorption: 3. Application to semiconductor-molecule assemblies,”
*Journal of Physical Chemistry B*, vol. 110, no. 50, pp. 25181–25190, 2006. View at Publisher · View at Google Scholar · View at PubMed · View at Scopus - W. R. Duncan and O. V. Prezhdo, “Theoretical studies of photoinduced electron transfer in dye-sensitized TiO
_{2},”*Annual Review of Physical Chemistry*, vol. 58, pp. 143–184, 2007. View at Publisher · View at Google Scholar · View at PubMed · View at Scopus - L. G. C. Rego and V. S. Batista, “Quantum dynamics simulations of interfacial electron transfer in sensitized TiO
_{2}semiconductors,”*Journal of the American Chemical Society*, vol. 125, no. 26, pp. 7989–7997, 2003. View at Publisher · View at Google Scholar · View at PubMed · View at Scopus - A. G. Agrios, K. A. Gray, and E. Weitz, “Narrow-band irradiation of a homologous series of chlorophenols on TiO
_{2}: charge-transfer complex formation and reactivity,”*Langmuir*, vol. 20, no. 14, pp. 5911–5917, 2004. View at Publisher · View at Google Scholar - S. Kim and W. Choi, “Visible-light-induced photocatalytic degradation of 4-chlorophenol and phenolic compounds in aqueous suspension of pure titania: demonstrating the existence of a surface-complex-mediated path,”
*Journal of Physical Chemistry B*, vol. 109, no. 11, pp. 5143–5149, 2005. View at Publisher · View at Google Scholar · View at PubMed · View at Scopus - M. Bledowski, L. Wang, A. Ramakrishnan et al., “Visible-light photocurrent response of TiO
_{2}-polyheptazine hybrids: evidence for interfacial charge-transfer absorption,”*Physical Chemistry Chemical Physics*, vol. 13, no. 48, pp. 21511–21519, 2011. View at Publisher · View at Google Scholar · View at PubMed - R. A. Smith,
*Semiconductors*, Cambridge University Press, Cambridge, UK, 1959. - J. Tauc, R. Grigorovici, and A. Vancu, “Optical properties and electronic structure of amorphous germanium,”
*Physica Status Solidi*, vol. 15, no. 2, pp. 627–637, 1966. View at Google Scholar - P. K. Basu,
*Theory of Optical Processes in Semiconductors: Bulk and Microstructures*, Clarendon Press, Oxford, UK, 1997. - T. P. McLean, “The absorption-edge spectrum of semiconductors,” in
*Semiconductor Program*, A. F. Gibson, Ed., vol. 5, pp. 53–102, Heywood, 1960. View at Google Scholar - J. I. Pankove,
*Optical Processes in Semiconductors*, Prentience-Hall, Upper Saddle River, NJ, USA, 1971. - D. Dragoman and M. Dragoman,
*Optical Characterization of Solids*, Springer, Berlin, Germany, 2001. - P. Kubelka, “New contributions to the optics of intensely light-scattering materials,”
*Journal of the Optical Society of America*, vol. 38, no. 5, pp. 448–457, 1948. View at Google Scholar · View at Scopus - P. Kubelka, “New contributions to the optics of intensely light-scattering materials. Part II: nonhomogeneous layers,”
*Journal of the Optical Society of America*, vol. 44, no. 4, pp. 330–335, 1954. View at Google Scholar - P. Kubelka and F. Munk, “Ein Beitrag zur Optik der Farbanstriche,”
*Zeitschrift fuer technische Physik*, vol. 12, no. 11, pp. 593–601, 1931. View at Google Scholar - W. W. Wendlandt and H. G. Hecht, “Reflectance Spectroscopy,” in
*Chemical Analysis*, P. J. Elving and I. M. Kolthoff, Eds., vol. 21, p. 298, Interscience, New York, NY, USA, 1966. View at Google Scholar - A. P. Finlayson, V. N. Tsaneva, L. Lyons, M. Clark, and B. A. Glowacki, “Evaluation of Bi-W-oxides for visible light photocatalysis,”
*Physica Status Solidi (A) Applications and Materials*, vol. 203, no. 2, pp. 327–335, 2006. View at Publisher · View at Google Scholar · View at Scopus - W. W. Gärtner, “Depletion-layer photoeffects in semiconductors,”
*Physical Review*, vol. 116, no. 1, pp. 84–87, 1959. View at Publisher · View at Google Scholar · View at Scopus - M. A. Butler, “Photoelectrolysis and physical properties of the semiconducting electrode tungsten trioxide,”
*Journal of Applied Physics*, vol. 48, no. 5, pp. 1914–1920, 1977. View at Google Scholar - S.-E. Lindquist, A. Hagfeldt, S. Sodergren, and H. Lindstrom, “Charge transport in nanostructured thin-film electrodes,” in
*Electrochemistry of Nanomaterials*, G. Hodes, Ed., pp. 169–200, Wiley-VCH, Weinheim, Germany, 2001. View at Google Scholar - K. Leitner, J. W. Schultze, and U. Stimming, “Photoelectrochemical investigations of passive films on titanium electrodes,”
*Journal of the Electrochemical Society*, vol. 133, no. 8, pp. 1561–1568, 1986. View at Google Scholar · View at Scopus - U. Stimming, “Photoelectrochemical studies of passive films,”
*Electrochimica Acta*, vol. 31, no. 4, pp. 415–429, 1986. View at Google Scholar · View at Scopus - A. J. Nozik and R. Memming, “Physical chemistry of semiconductor-liquid interfaces,”
*Journal of Physical Chemistry*, vol. 100, no. 31, pp. 13061–13078, 1996. View at Google Scholar · View at Scopus - A. J. Bard, “Design of semiconductor photoelectrochemical systems for solar energy conversion,”
*Journal of Physical Chemistry*, vol. 86, no. 2, pp. 172–177, 1982. View at Google Scholar · View at Scopus - A. Hagfeld and M. Grätzel, “Light-induced redox reactions in nanocrystalline systems,”
*Chemical Reviews*, vol. 95, no. 1, pp. 49–68, 1995. View at Google Scholar - G. Hodes, I. D. J. Howell, and L. M. Peter, “Nanocrystalline photoelectrochemical cells. A new concept in photovoltaic cells,”
*Journal of the Electrochemical Society*, vol. 139, no. 11, pp. 3136–3140, 1992. View at Google Scholar · View at Scopus - A. Wahl, M. Ulmann, A. Carroy, and J. Augustynski, “Highly selective photo-oxidation reactions at nanocrystalline TiO
_{2},”*Journal of the Chemical Society, Chemical Communications*, no. 19, pp. 2277–2278, 1994. View at Publisher · View at Google Scholar · View at Scopus - J. J. Kelly and D. Vanmaekelbergh, “Charge carrier dynamics in nanoporous photoelectrodes,”
*Electrochimica Acta*, vol. 43, no. 19-20, pp. 2773–2780, 1998. View at Google Scholar · View at Scopus - R. Solarska, I. Rutkowska, R. Morand, and J. Augustynski, “Photoanodic reactions occurring at nanostructured titanium dioxide films,”
*Electrochimica Acta*, vol. 51, no. 11, pp. 2230–2236, 2006. View at Publisher · View at Google Scholar · View at Scopus - M. A. Butler and D. S. Ginley, “Prediction of flatband potentials at semiconductor-electrolyte interfaces from atomic electronegativities,”
*Journal of the Electrochemical Society*, vol. 125, no. 2, pp. 228–232, 1978. View at Google Scholar · View at Scopus - Y. Paz, “Preferential photodegradation—why and how?”
*Comptes Rendus Chimie*, vol. 9, no. 5-6, pp. 774–787, 2006. View at Publisher · View at Google Scholar · View at Scopus - M. Herrmann and H. P. Boehm, “Saure Hydroxylgruppen auf der Oberfläche,”
*Zeitschrift fuer Anorganische und Allgemeine Chemie*, vol. 368, pp. 73–86, 1969. View at Google Scholar - C. Kormann, D. W. Bahnemann, and M. R. Hoffmann, “Photolysis of chloroform and other organic molecules in aqueous TiO
_{2}suspensions,”*Environmental Science and Technology*, vol. 25, no. 3, pp. 494–500, 1991. View at Google Scholar - G. Nagasubramanian, B. L. Wheeler, and A. J. Bard, “Semiconductor electrodes XLIX. Evidence for fermi level pinning and surface-state distributions from impedance measurements in acetonitrile solutions with various redox couples,”
*Journal of the Electrochemical Society*, vol. 130, no. 8, pp. 1680–1688, 1983. View at Google Scholar - L. M. Peter, E. A. Ponomarev, and D. J. Fermín, “Intensity-modulated photocurrent spectroscopy: reconciliation of phenomenological analysis with multistep electron transfer mechanisms,”
*Journal of Electroanalytical Chemistry*, vol. 427, no. 1-2, pp. 79–96, 1997. View at Google Scholar · View at Scopus - D. Tafalla and P. Salvador, “Analysis of the photocurrent transient behaviour associated with flatband potential shifts during water splitting at n-TiO
_{2}electrodes,”*Journal of Electroanalytical Chemistry and Interfacial Electrochemistry*, vol. 270, no. 1-2, pp. 285–295, 1989. View at Google Scholar - J. J. Kelly and R. Memming, “The influence of surface recombination and trapping on the cathodic photocurrent at p-type [Group] III-V electrodes,”
*Journal of the Electrochemical Society*, vol. 129, no. 4, pp. 730–738, 1982. View at Google Scholar · View at Scopus - L. Kavan, M. Grätzel, S. E. Gilbert, C. Klemenz, and H. J. Scheel, “Electrochemical and photoelectrochemical investigation of single-crystal anatase,”
*Journal of the American Chemical Society*, vol. 118, no. 28, pp. 6716–6723, 1996. View at Publisher · View at Google Scholar · View at Scopus - W. Kang and M. S. Hybertsen, “Quasiparticle and optical properties of rutile and anatase TiO
_{2},”*Physical Review B*, vol. 82, no. 8, Article ID 085203, 2010. View at Publisher · View at Google Scholar · View at Scopus - M. C. Toroker, D. K. Kanan, N. Alidoust, L. Y. Isseroff, P. Liao, and E. A. Carter, “First principles scheme to evaluate band edge positions in potential transition metal oxide photocatalysts and photoelectrodes,”
*Physical Chemistry Chemical Physics*, vol. 13, no. 37, pp. 16644–16654, 2011. View at Publisher · View at Google Scholar · View at PubMed - Y. Wu, M. K. Y. Chan, and G. Ceder, “Prediction of semiconductor band edge positions in aqueous environments from first principles,”
*Physical Review B*, vol. 83, no. 23, pp. 235–301, 2011. View at Publisher · View at Google Scholar - D. Cahen and A. Kahn, “Electron energetics at surfaces and interfaces: concepts and experiments,”
*Advanced Materials*, vol. 15, no. 4, pp. 271–277, 2003. View at Publisher · View at Google Scholar · View at Scopus - K. Besocke and S. Berger, “Piezoelectric driven Kelvin probe for contact potential difference studies,”
*Review of Scientific Instruments*, vol. 47, no. 7, pp. 840–842, 1976. View at Publisher · View at Google Scholar · View at Scopus - L. Kronik and Y. Shapira, “Surface photovoltage phenomena: theory, experiment, and applications,”
*Surface Science Reports*, vol. 37, no. 1, pp. 1–206, 1999. View at Publisher · View at Google Scholar · View at Scopus - L. Kronik and Y. Shapira, “Surface photovoltage spectroscopy of semiconductor structures: at the crossroads of physics, chemistry and electrical engineering,”
*Surface and Interface Analysis*, vol. 31, no. 10, pp. 954–965, 2001. View at Publisher · View at Google Scholar · View at Scopus - D. Cahen, G. Hodes, M. Grätzel, J. F. Guillemoles, and I. Riess, “Nature of Photovoltaic Action in Dye-Sensitized Solar Cells,”
*Journal of Physical Chemistry B*, vol. 104, no. 9, pp. 2053–2059, 2000. View at Google Scholar · View at Scopus - A. Rothschild, Y. Komem, A. Levakov, N. Ashkenasy, and Y. Shapira, “Electronic and transport properties of reduced and oxidized nanocrystalline TiO
_{2}films,”*Applied Physics Letters*, vol. 82, no. 4, pp. 574–576, 2003. View at Publisher · View at Google Scholar · View at Scopus - S. Bastide, D. Gal, D. Cahen, and L. Kronik, “Surface photovoltage measurements in liquids,”
*Review of Scientific Instruments*, vol. 70, no. 10, pp. 4032–4036, 1999. View at Google Scholar · View at Scopus - F. Lenzmann, J. Krueger, S. Burnside et al., “Surface photovoltage spectroscopy of dye-sensitized solar cells with TiO
_{2}, Nb_{2}O_{5}, and SrTiO_{3}nanocrystalline photoanodes: indication for electron injection from higher excited dye states,”*Journal of Physical Chemistry B*, vol. 105, no. 27, pp. 6347–6352, 2001. View at Publisher · View at Google Scholar - H. R. Sprünken, R. Schumacher, and R. N. Schindler, “Evaluation of the flat-band potentials by measurements of anodic/cathodic photocurrent transitions,”
*Faraday Discussions of the Chemical Society*, vol. 70, pp. 55–66, 1980. View at Publisher · View at Google Scholar · View at Scopus - H. O. Finklea, “Semiconductor electrode concepts and terminology,”
*Studies in Physical and Theoretical Chemistry*, vol. 55, pp. 1–42, 1988. View at Google Scholar - Y. V. Pleskov, V. M. Mazin, Y. E. Evstefeeva, V. P. Varnin, I. G. Teremetskaya, and V. A. Laptev, “Photoelectrochemical determination of the flatband potential of boron-doped diamond,”
*Electrochemical and Solid-State Letters*, vol. 3, no. 3, pp. 141–143, 2000. View at Publisher · View at Google Scholar · View at Scopus - A. Podborska, B. Gaweł, Ł. Pietrzak et al., “Anomalous photocathodic behavior of CdS within the urbach tail region,”
*Journal of Physical Chemistry C*, vol. 113, no. 16, pp. 6774–6784, 2009. View at Publisher · View at Google Scholar - K. Vinodgopal, S. Hotchandani, and P. V. Kamat, “Electrochemically assisted photocatalysis: titania particulate film electrodes for photocatalytic degradation of 4-chlorophenol,”
*The Journal of Physical Chemistry*, vol. 97, no. 35, pp. 9040–9044, 1993. View at Google Scholar - D. Monllor-Satoca and R. Gómez, “Electrochemical method for studying the kinetics of electron recombination and transfer reactions in heterogeneous photocatalysis: the effect of fluorination on TiO
_{2}nanoporous layers,”*Journal of Physical Chemistry C*, vol. 112, no. 1, pp. 139–147, 2008. View at Publisher · View at Google Scholar - G. Rothenberger, D. Fitzmaurice, and M. Grätzel, “Spectroscopy of conduction band electrons in transparent metal oxide semiconductor films: optical determination of the flatband potential of colloidal titanium dioxide films,”
*Journal of Physical Chemistry*, vol. 96, no. 14, pp. 5983–5986, 1992. View at Google Scholar · View at Scopus - G. Redmond and D. Fitzmaurice, “Spectroscopic determination of flatband potentials for polycrystalline TiO
_{2}electrodes in nonaqueous solvents,”*Journal of Physical Chemistry*, vol. 97, no. 7, pp. 1426–1430, 1993. View at Google Scholar - D. Fitzmaurice, “Using spectroscopy to probe the band energetics of transparent nanocrystalline semiconductor films,”
*Solar Energy Materials and Solar Cells*, vol. 32, no. 3, pp. 289–305, 1994. View at Google Scholar · View at Scopus - E. Burstein, “Anomalous optical absorption limit in InSb,”
*Physical Review*, vol. 93, no. 3, pp. 632–633, 1954. View at Publisher · View at Google Scholar · View at Scopus - T. S. Moss, “The interpretation of the properties of indium antimonide,”
*Proceedings of the Physical Society Section B*, vol. 67, no. 10, article 306, pp. 775–782, 1954. View at Publisher · View at Google Scholar · View at Scopus - B. O'Regan, M. Grätzel, and D. Fitzmaurice, “Optical electrochemistry I: steady-state spectroscopy of conduction-band electrons in a metal oxide semiconductor electrode,”
*Chemical Physics Letters*, vol. 183, no. 1-2, pp. 89–93, 1991. View at Google Scholar · View at Scopus - J. Nelson, “Continuous-time random-walk model of electron transport in nanocrystalline TiO
_{2}electrodes,”*Physical Review B*, vol. 59, no. 23, pp. 15374–15380, 1999. View at Google Scholar · View at Scopus - F. Fabregat-Santiago, I. Mora-Seró, G. Garcia-Belmonte, and J. Bisquert, “Cyclic voltammetry studies of nanoporous semiconductors. Capacitive and reactive properties of nanocrystalline TiO
_{2}electrodes in aqueous electrolyte,”*Journal of Physical Chemistry B*, vol. 107, no. 3, pp. 758–768, 2003. View at Publisher · View at Google Scholar - J. Bisquert and A. Zaban, “The trap-limited diffusivity of electrons in nanoporous semiconductor networks permeated with a conductive phase,”
*Applied Physics A*, vol. 77, no. 3-4, pp. 507–514, 2003. View at Publisher · View at Google Scholar · View at Scopus - M. J. Cass, A. B. Walker, D. Martinez, and L. M. Peter, “Grain morphology and trapping effects on electron transport in dye-sensitized nanocrystalline solar cells,”
*Journal of Physical Chemistry B*, vol. 109, no. 11, pp. 5100–5107, 2005. View at Publisher · View at Google Scholar · View at PubMed · View at Scopus - M. Bailes, P. J. Cameron, K. Lobato, and L. M. Peter, “Determination of the density and energetic distribution of electron traps in dye-sensitized nanocrystalline solar cells,”
*Journal of Physical Chemistry B*, vol. 109, no. 32, pp. 15429–15435, 2005. View at Publisher · View at Google Scholar · View at PubMed · View at Scopus - A. M. Roy, G. C. De, N. Sasmal, and S. S. Bhattacharyya, “Determination of the flatband potential of semiconductor particles in suspension by photovoltage measurement,”
*International Journal of Hydrogen Energy*, vol. 20, no. 8, pp. 627–630, 1995. View at Google Scholar - M. F. Finlayson, B. L. Wheeler, N. Kakuta et al., “Determination of flat-band position of CdS crystals, films, and powders by photocurrent and impedance techniques. Photoredox reaction mediated by intragap states,”
*Journal of Physical Chemistry*, vol. 89, no. 26, pp. 5676–5681, 1985. View at Google Scholar - J. R. White and A. J. Bard, “Electrochemical investigation of photocatalysis at CdS suspensions in the presence of methylviologen,”
*Journal of Physical Chemistry*, vol. 89, no. 10, pp. 1947–1954, 1985. View at Google Scholar - G. Chen, J. M. Zen, F. R.F. Fan, and A. J. Bard, “Electrochemical investigation of the energetics of irradiated FeS
_{2}(pyrite) particles,”*Journal of Physical Chemistry*, vol. 95, no. 9, pp. 3682–3687, 1991. View at Google Scholar - D. Mitoraj and H. Kisch, “Analysis of electronic and photocatalytic properties of semiconductor powders through wavelength-dependent quasi-Fermi level and reactivity measurements,”
*Journal of Physical Chemistry C*, vol. 113, no. 49, pp. 20890–20895, 2009. View at Publisher · View at Google Scholar - B. O'Regan, M. Grätzel, and D. Fitzmaurice, “Optical electrochemistry. 2. Real-time spectroscopy of conduction band electrons in a metal oxide semiconductor electrode,”
*Journal of Physical Chemistry*, vol. 95, no. 26, pp. 10525–10528, 1991. View at Google Scholar